- Hot search：
ISO 5629-2017 pdf free download
ISO 5629-2017 pdf free download.Paper and board Determination of bending stiffness Resonance method
Papier et carton — Determination de Ia résistance a laflexion — Méthode par resonance.
Set the clamp into vibration and carefully pull the test piece through the clamp until the free end of the test piece goes into resonance. This point is characterized by maximum amplitude of vibration and maximum sharpness of visibility of the vibrating end of the test piece under stroboscopic illumination (5A).
Check that the edge of the test piece is still perpendicular to the edge of the clamp.
Measure, as accurately as possible, the length of test piece projecting past the edge of the clamp. This may be done by carefully cutting or marking the test piece at the clamp edge, removing it from the clamps and measuring its length using a steel rule or other suitable device. The accuracy of measurement of resonant length shall be within ±0.25 mm or ±0,5 %. whichever value is greater in the particular instance concerned.
Alternatively, if the instrument is fitted with a lower clamp coupled to a measuring scale, this may be used. If this is done, the measurement should be carried out in accordance with the manufacturer’s instructions, but it is essential that it should be checked that the test piece has not stretched significantly during the test and thus, that the length indicated by the scale is identical with the length of test piece protruding past the clamp.
Check if necessary, by further decreasing the projecting length, that the resonance point has been reached and that resonance is occurring with only one antinode, since it is possible to obtain resonance showing two antinodes and one node (see Eigure2).
For materials of very low grammage, it may be necessary to release the cbinping pressure while adjusting the projecting length to give resonance. For materials of higher grammage, it may be possible to make the final adjustment of the projecting length to obtain resonance by both pulling and pushing the test piece through the clamp. However, the clamping pressure should be applied while the state of resonance is checked.
Using the initial values obtained for resonant length as a guide. carry out the procedure given above to determine the resonant length of 10 test pieces in each of the desired directions.
9.3 Procedure B
9.3.1 Mean grammage
Determine the mean grammage of the sample in accordance with ISO 536.
9.3.2 Resonant length
Carry out the determination of resonant length as in 922.ISO 5629-2017 pdf free download.
All resources on this website are from the Internet. It is only for personal study and research. No one is allowed to use it for any commercial purpose. If you need, please buy the genuine standard. If there is any infringement of your copyright, please contact the webmaster in time, and I will correct it immediately.
- Maybe you like
- Latest Updates
- ISO 287-2009 pdf free download
- ISO 527-5-2009 pdf free download
- ISO 659-2009 pdf free download
- ISO 660-2009 pdf free download
- ISO 712-2009 pdf free download
- ISO 725-2009 pdf free download
- ISO 730-2009 pdf free download
- ISO 927-2009 pdf free download
- ISO 2041-2009 pdf free download
- ISO 3040-2009 pdf free download
- ISO 3506-2-2009 pdf free download
- ISO 3506-3-2009 pdf free download